HAL Id: hal-02348316
Submitted on 5 Nov 2019
is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaireHAL, est
destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Photo-induced phase transitions in ferroelectrics
Charles Paillard, Engin Torun, Ludger Wirtz, Laurent Bellaïche
To cite this version:
Charles Paillard, Engin Torun, Ludger Wirtz, Laurent Bellaïche. Photo-induced phase transi- tions in ferroelectrics. Physical Review Letters, American Physical Society, 2019, 123, pp.087601.
Charles Paillard,1, 2 Engin Torun,3 Ludger Wirtz,3 Jorge ´I˜niguez,4, 3 and Laurent Bellaiche1
1Department of Physics and Institute for Nanoscience and Engineering,
University of Arkansas, Fayetteville, Arkansas 72701, USA
2Laboratoire Structures, Propri´et´es et Mod´elisation des Solides, CentraleSup´elec,
UMR CNRS 8580, Universit´e Paris-Saclay, 91190 Gif-sur-Yvette, France∗
3Physics and Materials Science Research Unit, University of Luxembourg,
162a avenue de la Fa¨ıencerie, L-1511 Luxembourg, Luxembourg
4Materials Research and Technology Department,
Luxembourg Institute of Science and Technology (LIST),
Avenue des Hauts-Fourneaux 5, L-4362 Esch/Alzette, Luxembourg
Ferroic materials naturally exhibit a rich number of functionalities, which often arise from ther- mally, chemically or mechanically induced symmetry breakings or phase transitions. Based on Density Functional Calculations, we demonstrate here that light can drive phase transitions as well in ferroelectric materials such as the perovskite oxides lead titanate and barium titanate. Phonon analysis and total energy calculations reveal that the polarization tends to vanish under illumina- tion, to favor the emergence of non-polar phases, potentially antiferroelectric, and exhibiting a tilt of the oxygen octahedra. Strategies to tailor photo-induced phases based on phonon instabilities in the electronic ground state are also discussed.
Ferroelectric materials possess a spontaneous electric
polarization that is switchable by electric fields. Active
research in bandgap engineering  and unconventional
photovoltaic mechanisms [2–4] have prompted perovskite
oxide ferroelectrics as potential light absorbers to con-
vert light into electric , mechanical [6–8] or chemi-
cal energy , or for optical memory writing  and
non-destructive reading . Numerous works focused
on the photo-induced deformation of the unit cell with-
out apparent symmetry breaking . However, a recent
experimental work hinted at possible structural phase
transitions occurring in ferroelectric BaTiO3 nanowires
under illumination . Using first-principles calcula-
tions, we show that photo-induced phase transitions are
indeed possible in ferroelectrics such as barium and lead
titanates. In both cases, transitions to non-polar phases
are predicted. Furthermore, material engineering strate-
gies based on competing lattice instabilities are suggested
to tailor the critical concentration of photo-induced car-
riers at which the transition occurs, thus opening the
way to a rational design of materials exhibiting specific
properties under illumination.
ABO3perovskite oxides are versatile materials exhibit-
ing a wide range of properties (magnetism, polar distor-
tions, etc.). Their high symmetry reference structure (see
Fig. 1) is cubic with theBcation enclosed in an octahe-
dral cage of oxygens at the center, and theAcation at the
edges of the cube. Simple atomic displacement patterns
– e.g. as the octahedra tilts or electric dipoles sketched
in Fig. 1 – make it possible to obtain various symme-
try breakings and control the materials properties. For
convenience, here we denote the most relevant of such
distortions using a generalized and simplified Glazer no-
tation  αβγ/uα0vβ0wγ0, which is introduced in the
caption of Fig. 1.
Among perovskite oxides, barium titanate (BTO) and
lead titanate (PTO) are prototypical ferroelectric mate-
rials. They exhibit a number of phases [14, 15] associated
with lattice instabilities of the reference cubic phase .
The transitions between phases are commonly driven by
temperature [14, 15], pressure [17–19] or static electric
fields . Here, we demonstrate that light can also act
as a knob to control the crystal symmetry. Optical ma-
nipulation of ferroic materials has mainly focused on the
transient manipulation of the ferroic order parameter,
relying on non-thermalized photoexcited carriers  or
strong anharmonic phonon couplings . In contrast, we
presently describe the emergence of new phases caused by
modified lattice instabilities in the presence of thermal-
ized photo-excited carriers,i.e. the electrons lying at the
bottom of the conduction band (CB) and the equal num-
ber of holes sitting at the top of the valence band (VB)
of a semiconductor during illumination. To this end, we
usedab-initio calculations, detailed in the next section,
before examining the cases of barium and lead titanate
respectively. Finally, we discuss the origin of this phe-
nomenon and test design strategies for the engineering of
photo-induced phase transitions in ferroelectrics.
We performed Density Functional Theory (DFT) cal-
culations using the Abinit package software , with
the Projector Augmented Wave (PAW) method [24, 25].
We employ a 2×2×2 supercell (with respect to the 5-
atom pseudo-cubic perovskite cell) containing 40 atoms.
Thek-point mesh used was a Γ-centered 8×8×8 grid;
the plane-wave cut-off was 35 Ha. A Fermi-Dirac distri-
bution with 0.1 eV smearing was used to populate the
electronic states. The electronic density was considered
converged when the difference in the calculated forces be-
tween two Self-Consistent Field (SCF) steps was smaller
than 10−8 Ha.Bohr−1. The structural relaxation was
000/u+u+0- polar displacements
FIG. 1. Sketch of a 2×2×2 supercell in the paraelectric cubic reference structure 000/000. A and B cations are in black and blue, oxygens in red. The symmetry of a phase is denoted by (i)its oxygen octahedra tilt patternαβγ, whereα,βandγare either 0 (no tilt), ”+” (in-phase tilt) or ”−” (antiphase tilt) and represent whether the oxygen octahedra tilts around the first, second and third pseudocubic axis, respectively. Simi- larly, we denote the electric dipole pattern using a Glazer-like notationuα0vβ0wγ0, in whichu, v, wrepresent the magnitude of the dipole inside the perovskite 5-atom cell, andα0, β0and γ0describes whether dipole vectors [uvw] are aligned parallel (”+”) or antiparallel (”−”) when moving by one perovskite 5-atom cell along the first, second and third pseudocubic di- rection. Typical polar (000/00w+), antipolar (000/u+u+0−), in-phase (00c+/000) and antiphase tilt (00c−/000) displace- ment patterns are depicted using arrows.
stopped when all the forces on the atoms were smaller
than 5 ×10−7 Ha.Bohr−1 and all components of the
stress tensor smaller than 0.1 MPa. BTO was described
using the PBESol  exchange-correlation functional,
while the Local Density Approximation [27, 28] was em-
ployed to treat PTO. Photo-excited thermalized carriers
are mimicked using Fermi-Dirac distribution with two
quasi-Fermi levels µe and µh, as commonly used to de-
scribe photovoltaic effects in, for instance, p−n junc-
tions . As a result, during our DFT calculations, the
density is self-consistently converged under the constraint
of having ne=nph (and nh =nph) electrons (holes) in
the CB (VB). In other words, at each Self-Consistent
Field (SCF) iteration, the following system of equations
wk[1−f(εik,σ, µh)], (1) ne= X
wkf(εik,σ, µe), (2) is solved for µe and µh using a bisection algorithm.
In the above equation, wk is the weight of k-point k,
f(εik, µ) is the occupation number (Fermi-Dirac distri-
bution) of state with eigenvalueεik;σ denotes the spin.
Nv is the index of the highest valence band. We assume
that there is no closing of the gap during our constrained
DFT calculations, which is in practice observed for the
concentrations of photo-excited carrier pairsnph consid-
ered in this work.
Note that all structures considered in this work were
geometrically relaxed under the photo-excitation con-
straint mentioned above. The criteria for convergence
of the structural degrees of freedom are set to be the
same as in electronic ground state calculations.
Phonon calculations using the Phonopy package 
were performed in the dark and under excitation on the
cubic perovskite oxides using a 2×2×2 supercell after
the system was structurally relaxed. No analytic cor-
rection, and thus no LO-TO splitting was considered, as
the required Born effective charges cannot be calculated
in photo-excited cases.
We first calculated the phonon band structure of cu-
bic BTO in Figs. (2.a-d) for different concentrations of
photoexcited carriers nph. In the dark (nph = 0 e/f.u.,
Fig. (2.a)), the phonon dispersion exhibits imaginary
(negative in the figure) frequency modes characteris-
tic of lattice instabilities. The main instability, at Γ,
is responsible for the emergence of the polar order in
BTO , which goes from a high temperature cubic
000/000 structure to a ferroelectric tetragonal 000/00w+
phase below∼393 K, then to an orthorhombic structure
000/0v+v+ below ∼280-270 K and finally to a rhombo-
hedral 000/u+u+u+ phase below ∼183 K . Upon
increasing the number of photo-excited carrier pairs to
nph = 0.05 e/f.u. (in Fig. (2.b)), the frequencies of un-
stable modes along theX−M−Γ path get closer to real
(positive) values, the ferroelectric soft optical mode at Γ
becoming less unstable. Furthermore, fornph≥0.1 e/f.u.
(Figs. (2.c-d)) the cubic phase no longer exhibits unstable
phonon modes and isdynamically stable!
We calculated the energy (see Fig. (3.a)) of the four
phases naturally occurring in bulk BTO, 000/000 (green
squares), 000/00w+ (blue diamonds), 000/0v+v+ (vio-
let triangles) and 000/u+u+u+ (ground state at 0 K in
dark conditions, black dashed baseline). The rhombohe-
dral phase has the lowest energy for low concentrations of
photo-excited carriers (up to≈0.0375 e/f.u.), while the
tetragonal phase is slightly more stable at intermediate
concentrations (nph≈0.0375−0.1 e/f.u.). When the cu-
bic phase is dynamically stable (nph>0.1 e/f.u.), we find
accordingly that 000/000 is the lowest-energy structure,
which is confirmed by the disappearance of polar atomic
displacements and the cell shape distortions of all con-
sidered phases (see Supplementary Material ). The
predicted transition towards the 000/000 phase is con-
sistent with the experimental observation, in BTO, of a
downward shift of the Curie temperature under illumina-
tion . Besides, the flattening of the energy landscape
around 0.03 e/f.u. (≈5×1020e.cm−3) may be accompa-
nied by a monoclinic phase transition (see Supplemental
Γ X R M Γ R X M Γ 0
Γ X R M Γ R X M Γ 0
Γ X R M Γ R X M Γ 0
Γ X R M Γ R X M Γ 0
Γ X R M Γ R X M Γ
−5 0 5 10 15 20 25
Γ X R M Γ R X M Γ
−5 0 5 10 15 20 25
Γ X R M Γ R X M Γ
−5 0 5 10 15 20 25
Γ X R M Γ R X M Γ
−5 0 5 10 15 20 25
(a) (b) (c) (d)
(e) (f) (g) (h)
0.00 0.05 0.10 0.15
FIG. 2. (a-d) Phonon band structure in paraelectric cubic BTO and (e-h) PTO for different concentrations of photoexcited carrier pairsnph = 0.00 e/f.u. (a & e), nph = 0.05 e/f.u. (b & f),nph= 0.10 e/f.u. (c & g) andnph= 0.15 e/f.u. (d & h).
The polar Γ dominant instability in BTO becomes stabilized (i.e. positive and real frequency) fornph≥0.10 e/f.u., as shown in (c) and (d). In PTO, the polar instability at Γ is replaced by a non-polar tilted instability atM andR.
Material ). We note that such a critical concentration
would match recent observations of a monoclinic phase
in BTO nanowires under illumination [12, 33].
PTO exhibits a single transition from the non-polar
cubic 000/000 phase to the ferroelectric tetragonal
000/00w+ structure below 765 K . The phonon dis-
persion of the cubic phase fornph= 0 e/f.u. (Fig. (2.e))
exhibits one main polar instability at Γ, but also unstable
modes at theRandM points associated with octahedra
tilting 00−and 00+, respectively. The strength of the po-
lar instability at Γ decreases with increasing the number
of photo-excited carriers (see Figs. (2.e-h)) as in BTO.
However, it never totally disappears, indicating that fer-
roelectricity in PTO is more robust against photocarrier
generation. In contrast, the strengths of the tilting in-
stabilities at R and M are slightly enhanced, and they
become dominant fornph ≥0.1 (Figs. (2.g-h)), suggest-
ing a transition from a polar to a non-polar structure
with oxygen tilts under illumination.
Hence, we compute the energies of several prototypi-
cal phases upon illumination, as shown in Fig. (3.b). The
ferroelectric 000/00w+ phase, which is the ground state
in dark conditions, is the black dashed baseline, while the
cubic phase is plotted as green squares. We also plot a
rhombohedral polar− − −/u+u+u+ structure (navy cir-
cles) and its non-polar counterpart, a− − −/000 (navy
diamonds). We consider as well an orthorhombic phase
(violet triangles) with the − −0/u−u¯−0− antipolar dis-
placement pattern . A 00c−/000 non-polar tetrago-
nal phase is also calculated (gold triangles). According to
Fig. (3.b), the ferroelectric 000/00w+ phase is the most
stable up tonph≈0.125 e/f.u., the non-polar phase with
tilts becoming dominant beyond that point. Overall, the
antipolar − −0/u−u¯−0− phase is slightly more favor-
able (by 0.2-0.3 meV/f.u.) than the− − −/000 phase for
nph ≥0.125 e/f.u. Because of this small energy differ-
ence, it is impossible to predict with certainty the sym-
metry of PTO at large concentrations of photo-excited
carriers, and we can only reckon that this should be a
phase with oxygen tilts.
Unlike BTO, the polar atomic distortion in the
000/00w+ phase remains rather large under photo-
excitation (see Supplementary Material ). Moreover,
both the antipolar displacement (for the− −0/u−u¯−0−
phase) and the tilt angle (for − − −/000 and − −
0/u−u¯−0−) increase withnph. In contrast, the polar dis-
placements of the− − −/u+u+u+ phase disappear with
increasingnph, and it thus collapses into the− − −/000
phase, confirming that tilts and polarization are com-
peting order parameters in PTO [35, 36], illumination
tipping the balance towards the former.
Furthermore, calculations of minimum energy tran-
sition paths between phases (see Supplementary Mate-
rial ) show that − −0/u−u¯−0− and − − −/000 are
unstable in the dark; however, the 000/00w+ phase re-
mains metastable under illumination, drawing the pic-
ture of a first-order light-induced transition in PTO.
The large concentration of 0.125 e/f.u. needed to
destabilize the 000/00w+ phase in PTO is potentially
outside the reach of experiments, and certainly not de-
sirable for applications. We can try to improve this
situation by mixing PTO with an antiferrodistortive
0.00 0.05 0.10 0.15
nph (e/f.u.) 0
5 10 15
000/0+v+v+ 000/000 000/00w+
0.00 0.05 0.10 0.15
nph (e/f.u.) 0
− − −/000
− − −/u+u+u+
− −0/u−u¯−0− 00−/000
0.00 0.05 0.10 0.15
nph (e/f.u.) 0
5 10 15 20
− − −/000
− −0/u−u¯−0− 000/0+0+w+ 00−/000
FIG. 3. (a) Energy of different phases in BTO with respect to the 000/u+u+u+ structure (dashed dark line), which is the ground state in the dark. The tetragonal 000/00w+ and then the cubic 000 phase become more energetically favor- able. (b) Energy of different phases in PTO with respect to the 000/00w+ structure (dashed dark line), which is the ground state in the dark, showing that non-polar antiferrodis- tortive phases become more stable at large concentration of photo-excited carriers. (c) Energy of different phases in PSTO with respect to the rhombohedral − − −/u+u+u+ structure (dashed dark line), which is the lowest energy phase consid- ered when no carriers are excited.
material such as SrTiO3, and form the solid solution
(Pb1/2Sr1/2)TiO3 (PSTO) to favor the tilt instability
with respect to the polar one. As a proof of concept,
several phases of PSTO with rocksalt order were cal-
culated in Fig. (3.c). In particular, a polar rhombohe-
dral − − −/u+u+u+ phase (black dashed line) is the
ground state in the dark. The 000/00w+ (purple tri-
angles) and the high-symmetry cubic 000/000 phase (in
green squares) have increasing energy withnph. On the
contrary, the antipolar tilted phase− −0/u−u¯−0− (light
blue triangles) becomes the most stable phase above
nph = 0.05 e/f.u., thus supporting the proposed design
strategy to reduce the critical concentration for the polar-
From this work, it also becomes apparent that the fer-
roelectric instability can be hampered by the photogen-
eration of free carriers. Obviously, free carriers screen the
long-range Coulombic interaction responsible for the po-
lar order [37, 41], thus seemingly disfavoring polar phases
with respect to non-polar ones. This is consistent with
calculations [37, 41] and experiments  performed by
doping BTO with free electrons. The former predicted
the disappearance of the polar order in BTO at a concen-
tration of extra-electrons of≈0.1 e/f.u., which is exactly
the concentration of photo-excited carriers that stabilizes
the cubic phase in our calculations. We also note that the
destruction of the polar order in BTO and the large sta-
bility (and metastability) window of the 000/00w+phase
in PTO are consistent with the doping calculations per-
formed in Ref. . In addition, photoexcitation tends to
move electrons from O 2pstates to Tidstates, thus de-
stroying the covalent bonding that drives the ferroelectric
order  and favoring non-polar orders. Looking at the
evolution of interatomic force constants (IFCs; see Sup-
plementary Material ) under photoexcitation, shows
that(i)almost all IFCs are reduced in magnitude under
photoexcitation, and (ii) the most affected IFCs corre-
sponds to 4th nearest neighbors interaction,i.e. similar
atoms (Ti-Ti, O-O, etc.) interacting along the<100 >
cubic directions. This parallels the further stabilization
of the paraelectric phase under photoexcitation in the
incipient ferroelectric PbTe, which results from screen-
ing of the long-range Coulomb interactions by the redis-
tributed photoexcited carriers along the<100 >cubic
directions . From the evidence presented here, as well
as in other works involving doping and photoexcited cal-
culations [37, 38], electrostatic screening by photoexcited
carriers appears as a universal mechanism for ”dipole-
dipole driven” ferroelectric materials such as BTO .
In addition, the volume of most phases decreases with
increasing concentration of excited carriers in both BTO
and PTO, except that of the cubic 000/000 phase, which
increases instead (see Supplementary Material ). In-
terestingly, the decrease of volume of the polar phases
is consistent with the disappearance of the polar order,
and is reminiscent of the well-known [17–19] effect of hy-
drostatic compression; yet, the volume increase of the
cubic phase under illumination should in principle favor
the polar instabilities. Hence, our results suggest that the
behavior of the polar distortion upon illumination cannot
be understood solely in terms of a photo-induced volume
change , and that screening effects play a central role.
There are, however, potential limitations of this work,
since DFT is known to underestimate the quasi-particle
bandgap. Furthermore, excitonic effects are described
within a mean-field approximation using constrained
DFT to mimic excited states occupations. First, we per-
formedG0W0 calculations with the Yambo  pack-
age - using DFT input from Quantum Espresso [46, 47]
- in order to accurately describe the conduction and va-
lence bands (see Supplementary Material ). The cor-
rected band structure is overall not altered, except for
an almost rigid upshift of the conduction bands. This
shift slightly depends on the studied phase (with differ-
ences smaller than 100 meV between phases). The shift is
smaller for non-polar phases, therefore facilitating further
the light-induced transitions towards such latter states.
For BTO, we checked the robustness of our conclu-
sions by performing calculations of zone center phonons
of the cubic phase with hybrid DFT. We compare calcu-
lations performed with the semi-local PBEsol functional
and the hybrid HSEsol  functional. Both functionals
give similar lattice constants and similar frequency for
the imaginary frequency of the soft ferroelectric mode,
even though the band gaps are quite different (1.8 eV for
PBEsol and 3.4 eV, close to the GW value, for HSEsol).
Despite the very different band gaps, the phonon frequen-
cies as a function of the excited charge density evolve sim-
ilarly: we observe a stabilization of the soft mode at an
excited charge density of 0.09 electron per formula unit
(see Supplementary Material ). Hence, although our
DFT-based description may slightly alter the critical con-
centrations at which transitions occur, the present qual-
itative behavior should be correct, especially given our
results in Fig. 2 for the dynamical lattice instabilities of
theparaelectric cubic state.
At last, let us discuss the possibility of having photo-
induced phase transitions to (small self-trapped, or ST)
polaronic states. Recent (doping) calculations have
shown that ST holes were unlikely in PTO [49, 50], but
could potentially be stabilized in cubic BTO . In
order to check the appearance of polaronic states, we
ran calculations in BaTiO3 under photoexcitation with
nph = 0.075 e/f.u. andnph = 0.150 e/f.u (with no sym-
metry). No trace of polaronic states was found.
In conclusion, we have shown that light absorption is
a viable route to switch on/off specific lattice instabili-
ties in complex materials such as ferroelectric perovskite
oxides. Via first-principles calculations we have demon-
strated the microscopic mechanism leading to a light-
controlled stabilization of the cubic phase in BTO but
not in PTO. The calculations are a promising tool to en-
gineer and optimize such light-triggered transformations,
suggesting strategies for their practical realization in suit-
ably chosen materials. The results presented in this work
could offer a route to design light-controlled memory, by
accessing light-induced metastable states (see Fig. 4 in
the Supplemental Material  and related discussion).
C. P. and L. B. thank the ARO grant W911NF-
16-1-0227. We also acknowledge support from the
National Research Fund, Luxembourg through project
INTER/ANR/13/20/NANOTMD (E. T. and L. W.)
and the intermobility program (Grant No. 15/9890527
Greenox, J. I. and L. B.). C. P. thanks the AHPCC and a
DoD challenge grant for use of computing resources. We
thank B. Dkhil and P. Ruello for interesting discussions.
 I. Grinberg, D. V. West, M. Torres, G. Gou, D. M. Stein,
L. Wu, G. Chen, E. M. Gallo, A. R. Akbashev, P. K.
Davies, J. E. Spannier, A. M. Rappe, Nature 503, 509
 B. I. Sturman, V. M. Fridkin, The Photovoltaic and
Photorefractive Effects in Noncentrosymmetric Materi-
als, Gordon and Breach Science Publishers (1992).
 L. Z. Tan, F. Zheng, S. M. Young, F. M. Wang, S. Liu, A.
M. Rappe,npj Computational Materials2, 16026 (2016).
 C. Paillard, X. Bai, I. C. Infante, M. Guennou, G. Gen-
este, M. Alexe, J. Kreisel, B. Dkhil,Advanced Materials
28, 5153 (2016).
 R. Nechache, C. Harnagea, S. Li, L. Cardenas, J.
Chakrabartty, F. Rosei,Nature Photonics9, 61 (2014).
 B. Kundys, M., Viret, D., Colson, D. O. Kundys,Nature
Materials9, 803 (2010).
 M. Lejman, G. Vaudel, I. C. Infante, P. Gemeiner, V. E.
Gusev, B. Dkhil, P. Ruello,Nat. Commun.5, 4301 (2014).
 B. Kundys,Applied Physics Reviews 2, 011301 (2015).
 Y. Cui, J., Briscoe, S. Dunn,Chemistry of Materials25,
 V. Iurchuk, D. Schick, J. Bran, D. Colson, A. Forget, D.
Halley, A. Koc, M. Reinhardt, C. Kwamen, N. A. Morley,
M. Bargheer, M. Viret, R. Gumeniuk, G. Schmerber, B.
Doudin, B. Kundys,Physical Review Letters117, 107403
 R. Guo, L. You, Y. Zhou, Z. S. Lim, X. Zou, L. Chen,
R. Ramesh, J. Wang, Nature Communications 4, 1990
 Y.-H. Kuo, S. Nah, K. He, T. Hu, A. M. Lindenberg,
Journal of Material Chemistry C 5, 1522 (2017).
 A. M. Glazer,Acta Crystallographica B28, 3384 (1972).
 G. H. Kwei, A. C. Lawson, S. J. L. Billinge, S. W.
Cheong, S. W. The Journal of Physical Chemistry 97,
 G. Shirane, S. Hoshino,Journal of the Physical Society
of Japan6, 265 (1951).
 P. Ghosez, E. Cockayne, U. V. Waghmare, K. M. Rabe,
Physical Review B 60, 836 (1999).
 I. A. Kornev, L. Bellaiche, P. Bouvier, P.-E. Janolin,
B. Dkhil, J. Kreisel,Physical Review Letters 95, 196804
 P.-E. Janolin, P. Bouvier, J. Kreisel, P. A. Thomas, I.
A. Kornev, L. Bellaiche, W. Crichton, M. Hanfland, B.
Dkhil,Physical Review Letters 101, 237601 (2008).
 M. Ahart, M. Somayazulu, R. E. Cohen, P. Ganesh, P.
Dera, H.-k. Mao, R. J. Hemley, Y. Ren, P. Liermann &
Z. Wu,Nature451, 545 (2008).
 H. Moriwakeet al.,J. Appl. Phys.119, 064102 (2016).
 A. Kirilyuk, A. V. Kimel, T. Rasing, Rev. Mod. Phys.
6 82, 2731 (2010).
 A. Subedi,Phys. Rev. B 92, 214303 (2015)
 X. Gonzeet al. Computational Physics Communications
180, 2582 (2009).
 P. E. Bl¨ochl,Physical Review B 50, 17953 (1994).
 M. Torrent, F. Jollet, F. Bottin, G. Z´erah, X. Gonze,
Computational Material Science 42, 337 (2008).
 J. P. Perdew, A. Ruzsinszky, G. I. Csonka, O. A. Vydrov,
G. E. Scuseria, L. A. Constantin, X. Zhou, K. Burke,
Physics Review Letters 100, 136406 (2008).
 W. Kohn, L. J. Sham, Physical Review 140, A1133
 J. P. Perdew, Y. Wang, Physical Review B 45, 13244
 P. W¨urfel, U. W¨urfel,Physics of Solar Cells: From Basic
Principles to Advanced Concepts, Wiley-VCH (2009).
 A. Togo, I. Tanaka,Scripta Materialia 108, 1 (2015).
 See Supplementary Material at ... for more details which
includes Refs. [12, 14, 17–19, 37, 42, 43, 45–48, 51?
? –58]. We detail the symmetry and atomic displace-
ment evolution under excitation of carriers; Nudge Elas-
tic Band calculations show that the transition is likely
to be first order and that the non-polar phase are not
metastable, but rather unstable; we discuss the occur-
rence of a monoclinic phase in BaTiO3; Volume changes
under illumination are compared with hydrostatic pres-
sure results from the literature. The evolution of Inter-
atomic Force Constants is also depicted. Finally, via the
GW-approximation and hybrid DFT calculations, we dis-
cuss the relevance of many-body effects for the photo-
iduced stabilization of the cubic phase.
 L. Belyaev, V. M. Fridkin, A. A. Grekov, N. A. Kosono-
gov, A. I. Rodin,Le J. Phys. Colloq.33, C2-123 (1972).
 Pump-probe experiments on BiFeO3 in Ref.  estimate
nph ∼ 5×1019e cm−3 with maximum used fluences
of ∼50µJ.cm−2. In Ref.  (which observes a mono-
clinic phase in BaTiO3nanowires) fluences ranging up to
600µJ.cm−2 are used, which would correspond to a car-
rier concentration of ∼ 60050.5×1019 ≈6×1020e cm−3.
This order of magnitude matches the region where we
observed flattening of the energy landscape in Fig. 3a
(around the 000/u+u+u+to 000/00w+transition) which
could potentially harbor a monoclinic phase as discussed
in the Supplementary Material .
 L. Bellaiche, J. ´I˜niguez, Physical Review B 88, 014104
 I. A. Kornev, L. Bellaiche, P.-E. Janolin, B. Dkhil, E.
SuardPhysical Review Letters 97, 157601 (2006).
 J. C. Wojde l, P. Hermet, M. P. Ljungberg, P. Ghosez,
J. ´I˜niguez, Journal of Physics: Condensed Matter 25,
 H. J. Zhao, A. Filippetti, C. Escorihuela-Sayalero, P.
Delugas, E. Canadell, L. Bellaiche, V. Fiorentini, and
J. ´I˜niguez,Physical Review B 97, 054107 (2018).
 M.P. Jiang, M. Trigo, I. Savi´c, ´E. D. Murray, C. Bray,
J. Clark, T. Henighan, M. Kozina, M. Chollet, J. M.
Glownia, M. C. Hoffmann, D. Zhu, O. Delaire, A. F.
May, B. C. Sales, A. M. Lindenberg, P. Zalden, T. Sato,
R. Merlin, D. A. Reis,Nat. Commun.7, 12291 (2016).
 A. Filippetti, V. Fiorentini, F. Ricci, P. Delugas, J.
´I˜niguez,Nat. Commun.7, 11211 (2016).
 R. E. Cohen,Nature 358, 136 (1992).
 Y. Wang, X. Liu, J. D. Burton, S. S. Jaswal, E. Y. Tsym-
bal,Physical Review Letters 109, 247601 (2012).
 J. Fujiokaet al.,Scientific Reports5, 13207 (2015).
 C. Paillard, S. Prosandeev, L. Bellaiche,Physical Review
B 96, 045205 (2017).
 M. S. Hybertsen, S. G. Louie, Phys. Rev. B 34, 5390
 Marini, A., Hogan, C., Gr¨uning, M. & Varsano, D.
Yambo: An ab initio tool for excited state calculations.
Comput. Phys. Commun.180, 1392–1403 (2009).
 Giannozzi, P.et al.QUANTUM ESPRESSO: a modular
and open-source software project for quantum simula-
tions of materials.J. Phys. Condens. Matter 21, 395502
 Giannozzi, P.et al. Advanced capabilities for materials
modelling with Quantum ESPRESSO.J. Phys. Condens.
Matter 29, 465901 (2017).
 L. Schimka, J. Harl, G. Kresse, J. Chem. Phys. 134,
 P. Erhart, A. Klein, D. ˚Aberg, B. Sadigh,Phys. Rev. B
90, 035204 (2014).
 C. Paillard, G. Geneste, L. Bellaiche, B. Dkhil,J. Phys.
Condens. Matter 29, 485707 (2017).
 H. D. Megaw,Acta Crystallographica5, 739 (1952).
 E. Weinan, W. Ren, E. Vanden-Eijnden,J. Chem. Phys.
126, 164103 (2007).
 Z.-G. Ye, B. Noheda, M. Dong, D. E. Cox, G. Shirane,
Physical Review B 64, 184114 (2001).
 L. Bellaiche, A. Garc´ıa, D. Vanderbilt,Physical Review
Letters 84, 5427 (2000).
 D. Sangalli, A. Ferretti, H. Miranda, C. Attaccalite, I.
Marri, E. Cannuccia, P. Melo, M. Marsili, F. Paleari,
A. Marrazzo, G. Prandini, P. Bonf`a, M.O. Atambo, F.
Affinito, M. Palummo, A. Molina-S´anchez, C. Hogan, M.
Gr¨uning, D. Varsano, A. Marini, arXiv:1902.03837 [cond-
 C. Thomsen, H.T. Grahn, H.J. Maris, and J. Tauc,Phys.
Rev. B 34, 4129 (1986).
 R. Dovesi, A. Erba, R. Orlando, C. M. Zicovich-Wilson,
B. Civalleri, L. Maschio, M. Rerat, S. Casassa, J. Baima,
S. Salustro, B. Kirtman, WIREs Comput Mol Sci. 8,
 G. Sophia, P. Baranek, C. Sarrazin, M. Rerat, R. Dovesi,
Phase Transitions: A Multinational Journal, 81, 1069-